Download presentation

Published byCody Simmons Modified over 4 years ago

1
**Buckling Delamination with Application to Films and Laminates**

Thermal gradient with interruption of heat transfer across crack. No crack driving force due to film stress; Unless Mixed mode interface crack Compression in film producing buckling Buckling delamination Show Volinsky movie

2
**Mechanics of thin films and multilayers **

Application areas electronics, coatings of all kinds. Example: Buckle Delaminations Good Delaminations on Patterned substrates

3
**Thermal Barrier Coatings (TBCs) **

Application to jet and power generating turbines Ceramic (Zirconia) Ceramic (Alumina) Metal bond coat Blades taken from an engine showing areas of spalled-off TBC

4
**Buckle Delaminations: Interface cracking driven by buckling**

Three Morphologies: Straight-sided, Varicose and Telephone Cord Computer simulations Experimental observations 200nm DLC film on silicon Straight-sided Propagation of a buckle delamination along a pre- patterned tapered region of low adhesion between film and substrate. In the wider regions the telephone cord morphology is observed. It transitions to the straight-sided morphology in the more narrow region and finally arrests when the energy release rate drops below the level needed to separate the interface.

5
**A Model Problem—Mode I Buckling Delamination of Symmetric Bi-layer**

buckled state unbuckled state This neglects the very slight increase of P as the buckling amplitude increases Buckling stress of clamped beam length 2b. w is the width perpendicular to the plane. Overall buckling of the entire laminate (with thickness 2h) will not occur if b>L/4. unbuckled buckled Fixed b two crack tips

6
**Mode I Buckling Delamination of Symmetric Bi-layer: continued**

The energy release rate G can be re-written in the following non-dimensional form: unbuckled

7
**Abbreviated Analysis of the Straight-Sided Buckle Delamination **

A 1D analysis based on vonKarman plate theory (Derived in Class) Propagation direction Film pre-stress h Average stress in buckled film: In-plane compatibility condition Buckle deflection: Buckle amplitude: At edge of buckle: Energy release rate along propagating front Energy release rate and mode mix along sides from basic solution: Energy-release rate can also be obtained from direct energy change calculation Mode mix depends on the amplitude of The buckle Plots are given on next overhead

8
**if you can. It makes life easier!**

BASIC ELASTICITY SOLUTION FOR INFINITE ELASTIC BILAYER WITH SEMI-INFINITE CRACK (Covered in earlier lecture) Equilibrated loads. General solution for energy release rate and stress intensity factors available in Suo and Hutchinson (1990) Infinitely thick substrate-- Primary case of interest for thin films and coatings on thick substrates moment/length Dundurs’ mismatch parameters for plane strain: force/length delamination crack interface For homogeneous case: If both materials incompressible: is the more important of the two parameters for most bilayer crack problems Take if you can. It makes life easier!

9
**Basic solution continued:**

Energy release rate delamination crack interface Stress intensity factors: (see Hutchinson & Suo (1992) if second Dundurs’ parameter cannot be taken to be zero) where is shown as a plot and is tabulated in Suo & Hutch. Note: For any interface crack between two isotropic materials, no mismatch

10
**Interface toughness—the role of mode mix**

Experimental finding: The energy release rate required to propagate a crack along an interface generally depends on the mode mix, often with larger toughness the larger the mode II component. A phenomenological interface toughness law Liechti & Chai (1992) data for an epoxy/glass interface.

11
**Half-width of straight-sided delamination**

Energy release rate and mode mix on sides of Straight-sided buckle delamination Stress at onset of buckling Half-width at onset of buckling Energy/area available for release in planes strain Half-width of straight-sided delamination Impose: Stable configurations (half-widths, b) of 1D delaminations See earlier slide for interface toughness function Mode II Caution! This plot is difficult to interpret because each axis depends on

12
**Inverse determination of interface toughness, stress (or modulus) **

by measuring buckling deflection and delamination width Straight-sided delamination without ridge crack on flat substrate front (SS) The basic results can be written as: side Applies to any multilayer film with arbitrary stress distribution If bending and stretching stiffness of the film are known, then the energy release rates and the resultant pre-stress can be determined by measurement of the deflection and the delamination width. If resultant pre-stress is known, then the equations can be used to determine film modulus and release rates in terms of deflection and delamination width– see Faulhaber, et al (2006) for an example.

Similar presentations

© 2020 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google